O R I G I N A L P A P E R
Selective Conversion of Ethane to Ethene via Oxidative
Dehydrogenation Over Ca-doped ThO2
Tinku Baidya• Niels van Vegten• Alfons Baiker
Published online: 6 August 2011
Ó Springer Science+Business Media, LLC 2011
Abstract Ca-doped ThO2, synthesized by solution
com-bustion method was tested for dehydrogenation of ethane with CO2. Doping ThO2with Ca resulted in the creation of
oxide ion vacancies and an increased conversion of ethane compared to pure ThO2. On Th0.75Ca0.25O2selectivity to
ethene was 97 at 46% ethane conversion at 725°C. Well-known reference catalysts like 5%Cr/TS-1 or OMS-2 showed significantly lower selectivity, but the former was more active under the same conditions.
Keywords Oxidative dehydrogenation Ethane Ethene CO2 Solid solution Thorium oxide Ca doping
Ethane is the second major component of natural gas, which makes it a potential source of chemicals such as light olefins, oxygenates and aromatic hydrocarbons . Con-verting the abundant ethane to ethylene at low temperature has been a challenge in chemical and petrochemical industry for many years .
Oxidative dehydrogenation (ODH) is the simplest pro-cess of partial oxidation of light alkanes. A number of catalysts, mainly vanadium, molybdenum and other group V-based oxides have been studied as active catalyst in presence of O2 as oxidant [3–8]. Mechanistic findings
showed that V–O–S or Mo–O–S type of bridging bonds were responsible for the dehydrogenation [9, 10]. These
catalysts are not as active as would be required for use in large scale production. Since oxygen is a strong oxidant, high temperature cannot be used because selectivity decreases dramatically .
The use of N2O as alternative oxidation agent is troubled
by the fact that selectivity can be deteriorated at higher conversion due to the formation of reactive O: radical species from N2O [12, 13]. Furthermore, N2O also faces
the drawback of limited availability for any mass produc-tion of ethene. Recently, attempts have been made to uti-lize less reactive carbon dioxide as an oxidant for dehydrogenation of ethane to yield ethene [14, 15]. The advantage of utilization of the green house gas CO2 as
oxidant is that it might lead to higher selectivity at elevated temperatures because it is less prone to supply oxygen species for reaction. Furthermore, syngas can be obtained as a by-product of this process . The main problem encountered in this reaction is catalyst deactivation due to carbon deposition and thus termination of syngas produc-tion. Up to date, Mo2C/SiO2, Cr/H-ZSM-5 [18, 19],
Cr/TS-1, Cr/SiO2, Ga/TiO2, and CeO2-based
oxides  have been used in the dehydrogenation of ethane with CO2 as an oxidant. Among these catalysts,
chromium-based catalysts have proven to be the most active for this reaction. Chromium based catalysts sup-ported on TS-1 or Cr/H-ZSM-5 show best performance, but their reaction temperature is limited to about 650°C, since at higher temperatures selectivity decreases significantly .
To our knowledge application of non-redox oxide materials for this reaction with CO2has not been reported
in the literature, probably because of their low propensity for dissociating CO2. We have observed in an earlier study
that Ca-doped ThO2is capable of producing oxygen
radi-cals , probably by virtue of p-type conductivity. These
T. Baidya N. van Vegten A. Baiker (&)
Institute for Chemical and Bioengineering, Department of Chemistry and Applied Biosciences, ETH Zurich, 8093 Ho¨nggerberg, HCI, Zu¨rich, Switzerland e-mail: firstname.lastname@example.org
radicals could be beneficial for partial oxidation of ethane. A mild oxidizing compound such as CO2could also
dis-sociate at these oxide ion vacancy sites, producing oxide ion radicals at elevated temperature. Thus, these materials may afford a more selective process than the strong oxidant Cr(VI). With this in mind, we have explored Ca-doped ThO2 as a catalyst for the oxidative dehydrogenation of
ethane with CO2.
2.1 Catalyst Preparation
The ThO2-based catalysts were prepared using a single step
solution combustion method . Stoichiometric amounts of Th(NO3)4 (Aldrich-Fine Chemicals, 99%), Ca(NO3)2
4H2O (Acros Organics, 99? %) and tartaric acid were
taken in a 300 mL crystallizing dish with water. Initially, the mixture was heated to make a transparent solution and then kept in the furnace at 500°C. After dehydration, ignition started and within a minute the oxide product was obtained. Subsequently, the samples were calcined at 800°C for 10 h to remove carbonaceous products.
Reference catalyst OMS-2 (octahedral molecular sieve) was prepared following the procedure described in the literature . MnCl24H2O (7.5 g) was dissolved in water
(50 mL). Air was bubbled into the Mn2?solution at a high flow rate. Then, an aqueous solution (80 mL) containing NaOH (20 g) was added dropwise to the solution for 30 min. After 6 h, a brown colored product was obtained which was filtered, washed, and transferred into a 1 M aqueous solution of KCl (250 mL) and stirred for 12 h at room temperature for ion exchange. The product was then filtered and washed with deionized water. The K-birnessite was dried in air at 80°C for 4 h and then placed in a furnace to calcine stepwise in air at 200, 400, 600, and 800°C for about 2 h at each temperature.
To prepare 5%Cr/TS-1, TS-1 was synthesized following the procedure reported in the literature . Two grams of Tween 20 (SIAL) were dissolved in 32 g of distilled water. This surfactant solution was added to 19.2 g of tetrapro-pylammonium hydroxide (TPAOH, 25% aqueous solution, Acros Organics) under mild stirring, which resulted in a clear transparent solution. To the above micellar solution, 36 g of tetraethyl orthosilicate (Aldrich) was added drop-wise under vigorous stirring which was continued for another 1 h. To this solution, 1.808 g of tetra n-butyl tita-nate (Acros Organics) in 9.12 g of isopropyl alcohol (IPA) was then added dropwise under vigorous stirring for another 1 h. Subsequently, the mixture was crystallized at 160°C for 18 h in an autoclave. The product was recov-ered by centrifugation, washed with distilled water and
dried (110°C, 12 h). Then, it was heated to 800 °C by stepwise increase at an interval of 200°C. Finally, the TS-1 was suspended in 50 cc water solution of (NH4)2CrO4
under continuous stirring and heated until total evapora-tion. The resulting material was calcinated at 600°C for 6 h.
2.2 Catalysts Characterization
X-ray diffractograms were recorded on a PANalytical X’Pert using Cu Ka (k = 1.541 A˚ ) radiation in step mode between 10 and 70° 2h with a step-size of 0.017 and 0.3 s/ step. Metallic Cu was used as an internal standard.
The Raman spectra of the ThO2 based oxides were
recorded in the 180° backscattering geometry, using a 532 nm excitation from a diode pumped frequency doubled Nd:YAG solid state laser (model GDLM-5015 L, Photop Suwtech Inc., China) and a custom-built Raman spec-trometer equipped with a SPEX TRIAX 550 monochro-mator and a liquid nitrogen cooled charge-coupled device (CCD; Spectrum One with CCD 3000 controller, ISA Jobin Yovn). Laser power at the sample was *8 mW, and a typical spectral acquisition time was 1 min. The spectral resolution chosen was 2 cm-1.
2.3 Catalytic Tests
The reactor set-up was a conventional gas flow system where ethane and carbon dioxide were co-fed over the catalyst. The catalyst was placed in a quartz U-tube reactor (ID 4.5 mm) which itself was placed inside a temperature controlled furnace. Typically, 400 mg of catalyst was diluted with 1000 mg of SiO2(white sand, Acros Organics)
and kept in place between two quartz wool plugs. The quartz wool before the bed acted as a pre-heating zone. Gas flows were regulated by mass flow controllers (Brooks Instrument B. V, model 5850E). The total flow was kept at 50 cc min-1, yielding a space velocity of 7500 cc gcat-1
h-1. The temperature was measured by a thermocouple well on the outer surface of the quartz reactor at the middle of the catalyst bed. Comparative tests were performed at 725 °C. The exhaust gas was analyzed using an on-line gas chromatograph with both TCD and FID detectors, which was connected to the reactor with heated stainless steel lines. The GC (Agilent Technologies, model 6890N) was equipped with a CarbonPLOT capillary column which allowed full separation of exhaust gas components such as CO, CO2, CH4, C2H4and C2H6. Each of the products was
calibrated against a calibration gas mixture. Note that in some experiments small amounts (1–2%) of C3H6 and
C3H8were also observed over the Ca doped ThO2samples.
The carbon balance was 95% on an average in all experi-mental runs.
Ethane conversion (XC2H6) and selectivity to ethene
(SC2H4) are defined as:
XC2H6 (%) = (moles of C2H6 converted 9 100)/(moles
of C2H6in feed).
SC2H4(%) = (moles of C2H4in outlet gas 9 100)/(moles
of C2H6in feed).
CO2conversion (XCO2) and selectivity to CO (SCO) are
XCO2 (%) = (moles of CO2converted 9 100)/(moles of
SCO(%) = (moles of CO in outlet gas 9 100)/(moles of
3 Results and Discussion
3.1 Structural Characterization
The top panel in Fig.1 presents the XRD patterns of the ThO2 based catalysts. The XRD analysis shows that the
ThO2-based materials crystallized in the fluorite phase.
From the line broadening by applying the Scherrer formula, the crystallite sizes were calculated to be 15, 8 and 7 nm for ThO2, Th0.8Ca0.2O2 and Th0.75Ca0.25O2, respectively.
To check the shift in peak position due to Ca substitution in ThO2, X-ray diffraction was performed with a Cu internal
standard allowing accurate determination of the position of the Cu (111) reflection at 43.32 2h (JCPDS 4-0836). Its shift toward lower 2h values confirms the incorporation of larger Ca2? ions in the ThO2 lattice (Fig.1, bottom).
According to Vegard’s law of solid solutions, the lattice parameter changes depending on the size of the dopant ion. Thus, the shift could be attributed to the difference in ionic radii of the Ca2? (8 CN 1.12 A˚ ) ion compared to Th4? (8 CN 1.05 A˚ ). The larger the difference in ionic radii, the larger the shift of the (111) position will be. Since appar-ently Ca is incorporated in the ThO2, the catalysts can be
represented as Th1-xCaxO2.
Figure2 shows the XRD patterns of the reference catalysts. OMS-2 (octahedral molecular sieve) shows the byxbyite structure (Mn2O3, JCPDS 41-1442, Space group:
Ia-3). The reflections from chromium supported on SiO2
and TS-1 samples correspond to the presence of Cr2O3in
eskolaite phase (JCPDS 1-072-4555, Space group: R-3c). The sample color was green, which also confirmed the presence of Cr2O3.
Figure3a–e shows the Raman spectra of ThO2and
Ca-doped ThO2samples along with pure CaCO3and a mixture
of ThO2 and CaCO3. Raman spectra could give an
indi-cation of changes in the lattice due to Ca ion substitution in ThO2. The characteristic F2g symmetry peak at 465 cm-1
of ThO2is prominent. In Th0.8Ca0.2O2and Th0.75Ca0.25O2,
significant peak shift was not observed as ionic radii of Ca and Th ion are almost similar. This type of feature was not observed in CaCO3as well as in the mixture of ThO2and
CaCO3 (Fig.3b, c). A similar feature was observed for
CeO2, another fluorite structure, substituted with lower
valent rare earth metal ions, as reported by McBride et al.  and confirmed by several other groups [28–30]. They reported incorporation of various rare earth elements (RE) in CeO2forming Ce1-xRExO2-dsolid solutions in fluorite
structure and assigned the Raman band at *570 cm-1 to formation of oxide ion vacancies. This type of feature was not observed in CaCO3. The appearance of such a feature
in the Ca-doped ThO2 catalysts might therefore be an
indication of the presence of similar vacancies in the cur-rent systems. To confirm Ca substitution further, pure CaCO3 was also analyzed. Three characteristic vibration
modes, symmetric stretching (1084 cm-1), in-plane
Fig. 1 XRD analysis of ThO2, Th0.8Ca0.2O2 and Th0.75Ca0.25O2
(top), and magnified section of the XRD pattern of the (111) reflection of ThO2, Th0.8Ca0.2O2and Th0.75Ca0.25O2(bottom).#Indicates the
position of the reflections of the Cu standard used for these measurements
bending (712 cm-1) and lattice mode vibration (282 cm-1) are observed in CaCO3. These peaks are also observed
in CaCO3 and ThO2 mixture. Interestingly, the peaks at
282 cm-1 and 712 cm-1 are missing in the Ca doped samples indicating absence of bulk CaCO3. Moreover,
symmetric stretching peak is lowered from 1084 to 1072 cm-1and it becomes broad, which essentially means the loss of symmetry occurring due to the presence on surface. Therefore, Ca could be substituted in ThO2matrix
and they must be containing surface carbonate species due to basic in nature.
3.2 Catalytic Activity
The catalytic activity of the Ca-doped ThO2catalyst was
tested in the temperature range 600–750 °C (Fig.4) and varying C2H6/CO2ratios (Fig.5). Comparative data of the
catalytic performances of the Ca-doped ThO2catalysts and
the reference catalysts at a suitable reaction temperature of 725 °C are given Table1. In Fig.4 the temperature dependencies of conversion and selectivity to ethane of Th0.75Ca0.25O2catalysts are compared to those of the most
active reference catalyst 5%Cr/TS-1.
Fig. 2 XRD profiles of reference catalysts OMS-2 (Mn2O3,
octahe-dral molecular sieve), 10%Cr/SiO2 and 5%Cr/TS-1 * Indicates
reflections from Cr2O3
Fig. 3 Raman spectra of a CaCO3 b ThO2 c ThO2? CaCO3
dTh0.8Ca0.2O2and e Th0.75Ca0.25O2
Fig. 4 Temperature dependence of conversion of ethane and selec-tivity to ethene over Th0.75Ca0.25O2 and 5%Cr/TS-1 (reference
catalyst). Conditions: C2H6:CO2:Ar = 45:35:20%; Total flow—
50 cc/min, temperature—725°C; catalyst—0.4 and 1 g SiO2)
Fig. 5 Dependence of ethane conversion and selectivity to ethane on CO2/C2H6ratio over Th0.75Ca0.25O2. Conditions: Total flow—50 cc/
As emerges from Fig.4, ethane conversion over 5%Cr/ TS-1 was already over 30% at 600°C, while the Th0.75Ca0.25O2did not show any appreciable activity at this
temperature. However, over Ca/ThO2 the conversion
increased more strongly at higher temperatures reaching over 60% at 750°C. Selectivity to ethene was much higher over Th0.75Ca0.25O2being [97% in the whole temperature
range up to 725°C, while over the 5%Cr/TS-1 reference catalyst it decreased from 92% at 600°C to 74% at 725 °C. This behavior could indicate a different reaction mecha-nism on these catalysts. The role of Cr as active species has been elucidated in the literature . Ethene formation was shown to occur by reduction of Cr(VI) species and CO2
dissociates to re-oxidise Cr(III) to Cr(VI) under the reac-tion condireac-tions. Thus, dissociated oxygen is presumably more available over this catalyst compared to the Ca/ThO2
leading to lower selectivity at higher temperature. Th0.75Ca0.25O2cannot produce any oxidizing species like
CrVI= O. Compelling evidence for a different mechanism over Th0.75Ca0.25O2will be presented below.
The role of CO2is to generate oxygen species that take
part in the formation of ethene as well as to suppress car-bon deposition. The dependence of ethane conversion and selectivity to ethene on the ratio CO2/C2H6 is shown in
Fig.5. It shows that in the absence of CO2the selectivity
was 78% and it increased to [97% with increasing CO2/
C2H6ratio up to 1.5. Further increase in CO2did not show
Table1shows the catalytic results over the ThO2-based
catalysts along with the three reference catalysts OMS-2, 5%Cr/TS-1, and 10%Cr/SiO2. Note that at high
tempera-ture, thermal dehydrogenation as well as catalytic surface reaction contribute to the conversion of ethane. Significant thermal dehydrogenation of ethane occured above 700°C which generally lead to lower selectivity. This is confirmed by the experiment without catalyst (entry 1), where 39%
conversion at 83% selectivity to ethane was reached, without any detectable conversion of CO2. An optimum
temperature of 725 °C was selected for this comparative study to keep high selectivity to ethene at significant con-version of ethane. The selectivity was improved by using ThO2-based catalysts (entry 2). Surprisingly, conversion of
ethane decreased to 17% over pure ThO2, but selectivity
increased to more than 99%. 19% CO2was converted to
CO with a selectivity of about 95%. The higher conversion was regained by Ca incorporation up to 20–25 at.% into ThO2(entries 3–5). In absence of CO2(entry 4), the
con-version increased to 48% but selectivity went down to 78%. In presence of CO2(entry 3), conversion of ethane
remained at about 46% and selectivity was maintained at about 97% over Th0.75Ca0.25O2. The conversion of CO2
was more than 40% and CO, H2O and H2were obtained as
by-product. Selectivity to CO was found to be about 80%. Several reference catalysts OMS-2, 5%Cr/TS-1, and 10%Cr/SiO2 were studied for comparison showing
con-versions of 38, 74 and 31%, and selectivities of 82, 74 and 86%, respectively. Note that the most active catalyst, 5%Cr/TS-1, had significantly lower selectivity than Th0.75Ca0.25O2. It is an often made observation in oxidation
catalysis that the more active a catalyst, the less selective it is and vice versa. Interestingly, OMS-2 seems to be poorly active as catalyst because conversion and selectivity remained almost similar to that obtained without catalysts (compare entries 1 and 6). Only 13% conversion of CO2
was observed initially and it decreased to zero within 1 h without significant change in ethane conversion. This indicates that ethene formation over OMS-2 occurred mainly due to thermal dehydrogenation. Similarly, 10%Cr/ SiO2 showed very low conversion of CO2 within few
hours. However, 5%Cr/TS-1 showed a consistent conver-sion of CO2. Interestingly, selectivity to CO significantly
exceeded 100%. This could happen probably due to some
Table 1 Results of oxidative dehydrogenation of ethane over ThO2based catalysts along with reference catalysts
Entry Catalyst XC2H6 (%) SC2H4(%) XCO2 (%) SCO(%) Yield (%)
1 No catalyst 39 83 –a – 32 2 ThO2 17 [99 19 95 17 3 Th0.75Ca0.25O2 46 97 43 80 45 4 Th0.75Ca0.25O2b 48 78 – – 37 5 OMS-2 38 82 – – 31 6 5%Cr/TS-1 74 74 40 [100c 55 7 10%Cr/SiO2 31 86 – – 27
Conditions: C2H6:CO2:Ar = 45:35:20% for a total flow of 50 cc min-1at 725°C. A catalyst weight of 0.4 g was used along with 1 g of SiO2as
a No conversion detected
2H6:Ar:He = 40:20:40 (absence of CO2)
deep oxidation of hydrocarbons (ethane, ethene) to CO resulting in an apparent selectivity to CO higher than 100%.
At the temperatures employed in this study, ethane could crack under formation of carbonaceous residues on the catalyst surface . Since this coking would nega-tively influence the catalyst performance, the long term behavior of Th0.8Ca0.2O2was tested. A CO2/C2H6ratio of
1.3 was used for this experiment, instead of the 0.78 in the rest of the studies. Visual inspection showed the catalyst color to have changed from white to black, indicating some deposition of carbonaceous residues. However, as Fig.6 reveals, within the 25 h on stream, no significant changes in catalyst performance were observed. This testifies of a strong stability of the catalyst under reaction conditions, in spite of the color change observed.
Finally, it is interesting to speculate about the mecha-nism of the oxidative dehydrogenation process, albeit the elucidation of the mechanism was not in the focus of this work. Nevertheless the observed catalytic behavior allows some speculation. We have observed that dehydrogenation of ethane occurs in absence of catalyst at 725°C reaching a selectivity of about 83%. On the other hand, the reaction in the presence of Th1-xCaxO2afforded a selectivity of 97%,
although conversion remained almost unchanged in both cases.
Preliminary EPR measurements on the Th0.75Ca0.25O2
sample showed the genesis of paramagnetic oxygen species in the range of 3200–3600 Gauss after exposure to CO2at
725°C. These species could be removed after subsequent exposure to ethane. The loss of paramagnetic species due to ethane exposure hints towards a surface-bound radical oxygen species. In earlier work , it was found that
species were produced from O2 and were stabilized in
oxide ion vacancies available in Th0.8Ca0.2O2. Possibly,
disproportionation of CO2 on the Th0.75Ca0.25O2 catalyst
results in similar oxygen radical species. It seems feasible that is the common species, which could be produced from both reactants (O2or CO2) and get stabilized in the oxide
ion vacancy site. Based on the above results, it seems likely that a radical reaction mechanism (see below) is respon-sible for the selective reaction to ethene, but thermal dehydrogenation and cracking also contribute to conversion. € VO2, €VO:þ hþ CO2þ €VO:! CO þ O: C2H6þ O:! :C2H5þ OH OHþ hþ! :OH :C2H5þ :OH ! C2H4þ H2O or H2Oþ €VO:! H2þ O:
In the above mechanism, h?indicates a hole, €VO:and
VO2indicate the presence of one electron and no electron
in the oxide ion vacancy sites, respectively.
Activation of ethane and propane with O:was proposed in earlier studies leading the unsaturated analogs [33,34]. Formation of oxygen radical species from the dissociation of CO2is proposed in this work. However, as long as the
relevant oxygen species are not properly identified and their role is not elucidated, the reaction mechanism pro-posed above remains speculation.
Th1-xCaxO2solid solution catalysts were synthesized using
the solution combustion method and the presence of oxide ion vacancies was indicated by Raman spectroscopy. The catalysts were applied for the oxidative dehydrogenation of ethane with CO2in the temperature range 600–750°C and
afforded 97% selectivity to ethene at 46% ethane conver-sion. Ca-doping of ThO2 strongly improved the ethene
yield. Based on the results of experimental runs without catalyst and in the presence and absence of CO2as well as
preliminary EPR results we propose that the oxidative dehydrogenation occurs via both thermal dehydrogenation as well as a more selective radical pathway. The latter process seems to be dominant over Th0.75Ca0.25O2 under
the applied conditions.
Acknowledgments Financial support by ETH Zurich (TH-09 06-2) is kindly acknowledged. We thank Dr. Maxim Yulikov and Prof. Dr. Fig. 6 Long term behavior of catalyst Th0.8Ca0.2O2. Ethane
conver-sion and selectivity to ethene vs. time on-stream. Conditions: C2H6:CO2:Ar = 35:45:20%; total flow—50 cc/min, temperature—
Gunnar Jeschke (both ETH Zurich) for providing the EPR measure-ments and fruitful discussions.
1. Cavani F, Koutyrev M, Trifiro F (1996) Catal Today 28:319 2. Kung HH (1994) Adv Catal 40:1
3. Mamedov EA, Corberan VC (1995) Appl Catal A Gen 127:1 4. Blasco T, Nieto JML (1997) Appl Catal A Gen 157:117 5. Banares MA (1999) Catal Today 51:399
6. Heracleous E, Machli M, Lemonidou AA, Vasalos IA (2005) J Mol Catal A 232:29
7. Botella P, Dejoz A, Nieto JML, Concepcion P, Vazquez MI (2006) Appl Catal A Gen 298:16
8. Haddad N, Bordes-Richard E, Barama A (2009) Catal Today 142:215
9. Au CT, Chen KD, Dai HX, Liu YW, Luo JZ, Ng CF (1998) J Catal 179:300
10. Courtine P, Bordes E (1997) Appl Catal A Gen 157:45 11. Routray K, Reddy KRSK, Deo G (2004) Appl Catal A Gen
12. Ward MB, Lin MJ, Lunsford JH (1977) J Catal 50:306 13. Morales E, Lunsford JH (1989) J Catal 118:255
14. Takahara I, Chang WC, Mimura N, Saito M (1998) Catal Today 45:55
15. Wang S, Murata K, Hayakawa T, Hamakawa S, Suzuki K (2000) Appl Catal A Gen 196:1
16. Zhu J, Qin S, Ren S, Peng X, Tong D, Hu C (2009) Catal Today 148:310
17. Solymosi F, Nemeth R (1999) Catal Lett 62:197
18. Mimura N, Takahara I, Inaba M, Okamoto M, Murata K (2002) Catal Commun 3:257
19. Mimura N, Okamoto M, Yamashita H, Oyama ST, Murata K (2006) J Phys Chem B 110:21764
20. Zhao X, Wang X (2006) Catal Commun 7:633
21. Nakagawa K, Kajita C, Okumura K, Ikenaga N, Nishitani-Gamo M, Ando T, Kobayashi T, Suzuki T (2001) J Catal 203:87 22. Valenzuela RX, Bueno G, Solbes A, Sapina F, Martinez E,
Corberan VC (2001) Top Catal 15:181
23. Baidya T, van Vegten N, Jiang Y, Krumeich F, Baiker A (2011) Appl Catal A Gen 391:205
24. Patil KC, Aruna ST, Mimani T (2002) Curr Opin Solid State Mater Sci 6:507
25. Khomane RB, Kulkarni BD, Paraskar A, Sainkar SR (2002) Mater Chem Phys 76:99
26. Jin L, Reutenauer J, Opembe N, Lai M, Martenak DJ, Han S, Suib SL (2009) ChemCatChem 1:441
27. McBride JR, Hass KC, Poindexter BD, Weber WH (1994) J Appl Phys 76:2435
28. Banerji A, Grover V, Sathe V, Deb SK, Tyagi AK (2009) Solid State Commun 149:1689
29. Li SP, Lu JQ, Fang P, Luo MF (2009) J Power Sources 193:93 30. Askrabic S, Dohcevic-Mitrovic ZD, Radovic M, Scepanovic M,
Popovic ZV (2009) J Raman Spectrosc 40:650
31. Martinez-Ramireza S, Sanchez-Cortesa S, Garcia-Ramosa JV, Domingoa C, Fortesb C, Blanco-Varelab MT (2003) Cem Conc Res 33:2063
32. Heracleous E, Lemonidou AA (2004) Appl Catal A Gen 269:123 33. Alka K-I, Lunsford JH (1977) J Phys Chem 81:1393
34. Leveles L, Seshan K, Lercher JA, Lefferts L (2003) J Catal 218:307